Research Article Synthesis and Characterization of TiO ... · PDF file Polystyrene and...
Embed Size (px)
Transcript of Research Article Synthesis and Characterization of TiO ... · PDF file Polystyrene and...
Research Article Synthesis and Characterization of TiO2 Modified with Polystyrene and Poly(3-chloro-2-hydroxypropyl Methacrylate) as Adsorbents for the Solid Phase Extraction of Organophosphorus Pesticides
Enrique Alejo-Molina,1 A. Rafael Vilchis-Néstor,2
David Muñoz-Rodríguez,1 and Cristian Carrera-Figueiras1
1Cuerpo Académico de Quı́mica Fundamental y Aplicada, Facultad de Ingenieŕıa Quı́mica, Universidad Autónoma de Yucatán, Periférico Norte Km 33.5, Tablaje Catastral 13615, Colonia Chuburná de Hidalgo Inn, 97203 Mérida, YUC, Mexico 2Centro Conjunto de Investigación en Quı́mica Sustentable UAEM-UNAM, Carretera Toluca-Atlacomulco Km 14.5, Campus “El Rosedal”, San Cayetano, 50200 Toluca, MEX, Mexico
Correspondence should be addressed to Enrique Alejo-Molina; [email protected]
Received 16 January 2016; Revised 12 May 2016; Accepted 22 May 2016
Academic Editor: Jean-Marie Nedelec
Copyright © 2016 Enrique Alejo-Molina et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Novel hybrid TiO 2 particles were developed and assessed as an adsorbent for solid phase extraction (SPE) of organophosphorus
pesticides (fensulfothion, parathion methyl, coumaphos, and diazinon) from spiked water. The sol-gel method was used to synthesize TiO
2 particles, which were coated with free-radical polystyrene (PS) and poly(3-chloro-2-hydroxypropyl methacrylate)
(PClHPMA) polymers. Particle structures were determined via Fourier transform infrared spectroscopy to confirm that the polymers were successfully anchored to the TiO
2 particles. Thermogravimetric analysis was conducted to determine organic and
inorganicmatter in TiO 2 -PS andTiO
2 -PClHPMAparticles showing results of 20 : 80wt/wt% and 23 : 77wt/wt%, respectively. SEM-
EDS and X-ray diffraction test were conducted to determine the morphology and semielemental composition of the particles showing amorphous characteristics. By observing the contact angle, particles coated with PClHPMA were determined to be more hydrophilic than TiO
2 -PS particles. The pore size distributions obtained from the N
2 adsorption-desorption isotherms were
0.150 and 0.168 cm3g−1. The specific surface area (BET) was 239.9m2g−1 for TiO 2 -PS and 225.7m2g−1 for TiO
2 -PClHPMA. The
synthesized particles showed relatively high yields of adsorption in SPE. The pesticide recoveries obtained by high performance liquid chromatography ranged from 6 to 26% for TiO
2 -PClHPMA and 44 to 92% for TiO
Solid phase extraction (SPE) is a simple and versatile extrac- tion technique. It is an alternative to liquid-liquid extractions, and it permits the preconcentration of the sample with minimal risk of loss or contamination, retaining the desired component in a solid phase while the unwanted components of the matrix are eluted with a suitable solvent . SPE provides options for the development of new analytical protocols and has been utilized in food products (eggs, honey, milk, fish, and oranges) [2, 3] as well as different water
samples (tap water, surface water, mineral water, wastewater, groundwater, and run-off water) . Various analytes, such as dichlorodiphenyltrichloroethane (DDT) , heavy metals , polycyclic aromatic hydrocarbons (PAHs) , and pes- ticides [4, 8–14], have been extracted from different types of samples. Different techniques have been utilized to determine organophosphorus pesticides (OPPs), such as gas chromatog- raphy with flame photometric detector (GC–FPD) [9, 12], gas chromatography with flame ionization detector (GC–FID) , and high performance liquid chromatography with UV detector (HPLC-UV) [11, 13].
Hindawi Publishing Corporation Journal of Chemistry Volume 2016, Article ID 1289592, 11 pages http://dx.doi.org/10.1155/2016/1289592
2 Journal of Chemistry
Typically, the sorbents used for SPE have been mate- rials based on nonderivatized silica (silica gel, sand, and florisil) as well as silica bonded to organic functional groups such as the octyl (–C
8 ), octadecyl (–C
18 ), cyanopropyl
[–(CH 2 ) 3 CN], aminopropyl [–(CH
2 ) 3 NH 2 ], and phenyl
propyl groups; silica bonded to –C 8 or –C
18 is the most used
sorbent. Other reports have demonstrated the application of novel materials in SPE, such as carbon fibers , aluminum , polymeric materials [9, 12, 17], graphitized carbon black , and titanium dioxide (TiO
2 ) .
Titanium dioxide (TiO 2 ) is one of the most important
inorganic materials due to its potential applications in photo- catalysis, its ability for photoelectric conversion in solar cells, and its optical and adsorption properties.The surface of TiO
particles is particularly attractive for its application in SPE because it can act as a Lewis acid (Ti+) or a Bronsted-Lowry acid (Ti-OH) and interact with a variety of both organic and inorganic compounds . Therefore, the following compounds based on TiO
2 have been used as adsorbents in
SPE: TiO 2 particles have been used to preconcentrate organic
compounds andmetals [21–24], TiO 2 nanotubeswere applied
for the extraction of DDT and its metabolites , SiO 2 -
TiO 2 particles were tested for their adsorption of carcino-
genic metals  and nitrogen compounds , TiO 2 was
modified with dithizone for mercury adsorption , TiO 2
nanotubes coated with cetyltrimethylammonium bromide were applied in the solid phase microextraction (𝜇SPE) of a preconcentration of PAHs , and TiO
2 particles coated
with polyacrylonitrile were utilized as ion exchangers for metal extraction .However, the synthesis of aTiO
material modified with polystyrene (or poly(3-chloro-2- hydroxypropylmethacrylate)) and its application as a sorbent in SPE for the extraction of organophosphorus pesticides have not been reported.
The particles of metal oxides such as TiO 2 can be used
as sorbents without surface modification due to the presence of different types of titanol groups (Ti-OH). However, to increase their applicability and to modify their retention properties, the surface of such materials can be altered with immobilized organic phases to promote the inter- actions between the solid surface and organic molecules, such as van der Waals interactions, electrostatic attraction, donor-acceptor interactions, and chemisorption . Various organic compounds can be incorporated within the gel network via chemical bonds by the copolymerization of organic and inorganic precursors, for sol-gel processing.
Typically, the reagents tetraethylorthosilicate and alkox- ysilanes (or tetramethyl orthosilicate) are used as precursors in sol-gel synthesis. The polycondensation of alkoxysilanes is carried out at room temperature and can be described by three reactions: (i) hydrolysis, (ii) silanol condensation, and (iii) silanol-alcohol condensation. Sol-gel synthesis allows one to obtain materials with different physicochemical prop- erties, such as surface area, particle shape and size, porosity, and degree of functionalization, which are associatedwith the possibility of obtaining binary oxides and inorganic phases . With respect to SPE, the morphological andmechanical properties and, importantly, the chemical behavior of the
inorganic sorbent play a significant role in facilitating the immobilization of organic groups on the particle .
The aim of this work was the synthesis and characteriza- tion of two novel hybrid sorbents based on TiO
2 . The TiO
particles were synthesized through a sol-gel process followed by a free radical polymerization with polystyrene (PS) or poly(3-chloro-2-hydroxypropyl methacrylate) (PClHPMA). Both hybridmaterialswere analyzed by surface and structural characterization techniques. Additionally, the hybrid parti- cles were used to pack cartridges to evaluate their potential application as sorbents for the solid phase extraction of four organophosphorus pesticides (OPPs) from spiked water. The optimization of the SPE extraction is beyond the scope of this paper.
2. Materials and Methods
2.1. Materials. The reagents for hybrid polymer prepara- tion: vinyltrimethoxysilane (VTMOS), titanium isopropox- ide (IPT), benzoyl peroxide (BPO), 2,2-azobisisobutyronitrile (AIBN), styrene (S), and 3-chloro-2-hydroxypropyl metha- crylate (ClHPMA) and OPPs fensulfothion (FST), parathion methyl (MP), diazinon (DZN), and coumaphos (CMF), were obtained from Sigma-Aldrich (Saint Louis, MO, USA). Hydrochloric acid (HCl), tetrahydrofuran (THF), tolu- ene, acetone, ethanol, methanol, ammonium hydroxide (NH 4 OH), and acetonitrile (ACN) were purchased from J.
T. Baker (Phillipsburg, NJ, USA). All reagents were used as received without further purification.
2.2. Synthesis. Thesol-gelmethod reported by several authors was adapted for the synthesis of hybrid materials [33, 34].
The first step (Figure 1(a)) was the synthesis of TiO 2
particles functionalized with vinyl groups (TiO 2 -VTMOS).
Thirty-onemilliliters ofHClwasmixedwith 40mLof ethanol in a baker. Following this, 115mL of titanium isopropoxide (IPT) and 14.5mL of vinyltrimethoxysilane (VTMOS) were slowly added to the baker and stirred for 15min. Then, a solution of 30mL of H
2 O, 104mL of NH
4 OH, and 47mL of
ethanol was ad